The Sol-gel Preparation of Silica Gels
Embed Size (px)
Transcript of The Sol-gel Preparation of Silica Gels
Effect of Solvent Removal Experimental Procedure Caution: The following apparatus is assembled in the fume
Let us now consider what happens when the solvent is hood. The TEOS is added in the fumehad, and the sol-gel removed by evaporation to form xerogels. For polymer gels solution is stirred in the fume hod.
dense gel structure. When hydrolysis is more rapid (basecatalyzed gels), polymers are larger and more highly cross-linked. On impingement the polymers will not deform as readily due to removal of solvent from within the polymer. The gel dries to a more or less randomly packed array of identifiable particles around which are large voids.
far from gel point gel point xerOge' I ProperGes of the Dwgel
Figure 1. Acid-catalyzed hydrolysis. The method of removal of the solvent from the pores of the alcogel has a dramatic effect on the
SiQ particles solvent in pores
sol alcogel xerogel
4 iac B 9( *.
& $ - - a*@- & * @ %
far from gel point gel point xerogel
supercritcal drying in autoclave
properties of the drygel. Aerogels have very low densities and very good thermal insulating properties when sandwiched between glass plates and evacuated (6). Xerogels are denser than aerogels, have high surface areas, and are often microporous. They can be used as catalyst supports (7), ionic conductors (8) (when appro- priately doped), and precursors for a wide range of glasses, ceramics, coatings, films, and fibers,
air in pores
depending on the method of preparation. Figure 2. Base-catalyzed hydrolysis. There are also several commercialized proc-
esses of sol-gel technology, and an increasing conventional drying, such as evaporation, xerogels result. amount of research is being carried Out in this Ad- If it is removed via supercritieal evacuation, aerogels re. vanced applications are now rapidly evolving, including suit (5). ~h~~~ processes are illustrated schematically in synthesis of superconductors, coatings on optical memory Figure 3. disks, and large mirrors for laser weapons in space (9).
Figure 3. The sokgel process
such as these removal of solvent is expected to collapse the network, gradually resulting in additional cross-linking as unreacted -OH and-OR aouus come into contact. The dif- - . ferent structures of the slowly (acid-catalyzed) and rapidly (base-catalyzed) hydrolyzed gels respond differently to the
Preparation of Acid-Catalyzed Sols
Around-bottomed flask containing a magnetic stir bar is clamped by the neck above a magnetic stirrer, which is placed on a retort stand. (See Fig. 4.) The chemicals used were all reagent-grade and available from suppliers such as Fischer or Aldrich.
Approximately 30 mL of TEOS is poured into a 100-mL beaker (in the fume hood), and exactly 30 mL of TEOS from the beaker is measured out usim a graduated cylinder. This quantity is then pourei into the round-bottomed flask. Then 31 mL of etha- nol is measured out in a graduated cylinder and added to the TEOS in the flask. The solution should be briskly agitated using the magnetic stir har.
Then 38 mL of distilled water is mcasurrd out us- ing the graduated cylinder, and 3-4 drops of concen- trated HC1 is added to the water using a pipet. This acidic solution is poured into the TEOS solution in the flask, stirring all the time. The two solutions are initially immiscible but mix after a few minutes. The temperature of the solution is allowed to stabilize at
removal ofsolvent d G g drying. - High-density low-pore-volume gels are formed in weakly
cross-linked systems (acid-catalyzed gels). As the polymers impinge on one another they deform readily and form a Figure 4. Experimental setup for the preparation of silica sols.
600 Journal of Chemical Education
60 "C. The resulting pH of this acidic sol-gel solution should be about 3 and may be adjusted by adding more drops of acid as necessary
The sol-gel solution is left stirring for 1.5 h in the fume hood. The change in pH is not significant during the course of the sol-gel process, and adjustment of the pH is not re- quired. The molar ratio of TEOS:EtOH:H20 is calculated to be 1:4:16 using the following data. . mol wt TEOS = 208.33 g, density = 0.936 g/cm3
mol wt ethanol = 46.07 g, density = 0.789 &m3
Because the balanced equation for the hydrolysis of TEOS is
4 mol of water are required for complete hydrolysis. How- ever, excess water is used in this experiment to drive the reaction to the right. Previous experiments had shown that 16 mol of water allowed the sol-gel process to occur within a reasonable time period and produced monolithic gels.
The sol is poured into polythene tubes (about 5 or 6 tubes will be needed), and the lid is replaced tightly on one Sam- ple. The openings of the other samples are covered with clear plastic wrap, and each is secured with a rubber band. A few holes should be pierced in the wrap using a needle. Some samples are placed in the drying oven (60 'C), and one is left on the open bench.
The whole procedure may be repeated using a few drops of NKOH instead of HC1. The pH of the sol-gel solution should be about 9 in the alkaline case. The sol-gel solution may take longer to mix in the acid-catalyzed reaction. (Up to 2 h for reaction may be necessary.)
Obtaining the Alcogels
After 1 and 2 days the conditions of all the samples are reexamined. The samples in the oven should have gelled after 2 days (alcogels) and will move freely from the solu- tion in the tubes. Aproportion of these alcogel samples are removed from the oven, and their lids are tightly replaced. The remainder are left in the oven for up to 5 more days (7 days in total). Samples of acid- and base-catalyzed gels were placed in porcelain boat crucibles in a tube furnace
and converted to xerogels by heating in a stream of oxygen gas for 5 h at 500 "C.
Results and Discussion Physical Appearances
The physical appearances of the acid- and base-cata- lyzed xerogels are displayed in Figure 5. For both types of processing the sols contained in the tubes that were tightly sealed did not gel, nor did those that were covered with pierced plastic film and left at room temperature (Fig. 5a). However, if the acid- and base-catalyzed gels were covered with pierced plastic film and placed in an oven at 60 "C, alcogels were formed after 2 days (Fig. 5b) and had ap- proximately the same volume as the original sols. After 7 days in the oven, the alcogels in both cases had shrunk to about 25% of their former volumes (Fig. 5c, d).
In the wet alcogel the Si02 network surrounds the pores that are filled with EtOH and HzO. Because the gel is left in a drying oven, the solvent gradually evaporates, and the gel ages by additional cross-linking of unreacted -OH and -OR groups. This will cause the network to collapse some- what and result in a reduction in volume. However, the dried alcogel still contains residual -OH and -OR species as well as ROH and H20. If these are to be removed com- pletely to form a xerogel, the gel must be heated up to about 500 "C in an oxygen atmosphere.
Because the pore structure is somewhat collapsed in the dried alcogel relative to the wet alcogel, the porosity of the wet alcogel is expected to be much greater. The pore nature of the wet alcogel can be retained (before further shrinkage occurs in the oven) by supercritically drying the gel to form an aerogel.
Resolution of Particles The acid-catalyzed alcogel (Fig. 5c) is transparent,
whereas the base-catalyzed gel is opaque (Fig. 5d). The xerogels are similar in appearance to the alcogels but more shrunken. The physical appearances of the dried gels may be explained by their microstructures as obtained by transmission electron microscopy. Figures 6 and 7 show typical transmission electron microscope photographs of acid- and base-catalyzed xerogels.
The acid-catalyzed xerogels exhibit extremely fine mi- crostructural features, and the low electron density con- trast in the photograph of the xerogel sample suggests that
Figure 5. Physical appearance of (a) acid- or base-catalyzed sol, (b) acid-catalyzed alcogel after 2 days at 60 "C, (c) acid-catalyzed alco- gel after 7 days at 60 "C, (d) base-catalyzed alcogel after 7 days at 60 "C. Figure 6. Typical microstructure of an acid-catalyzed xerogel.
Volume 71 Number 7 July 1994 601
, .. - . , . ,. : formation of highly branched silica clusters that do not in- ,, , : tercomect before gelation. These clusters form relatively e:19 ,.'.., large polymers that grow at the expense of the deform or
shrink. Hence the gel dries as a random packed array of identifiable particles (Fig. 2). and silica xerogels prepared using base catalysis are expected to be particulate (Fig. 7).
However, acid catalysis favors a reduced rate of hydroly- sis, causing relatively small polymers. When these are dried, strong surface tension forces are generated by the removal of solvent from the small regions between the polymers. As these weakly cross-linked polymers impinge, they readily deform and produce a dense gel structure (Fig. 1). Hence the gels prepared from acid hydrolysis have extremely fine microstructural features and are micropor- ous (Fig. 6).
Figure 7. Typical microstructure of a base-catalyzed xerogel. The authors would like to thank the Dreyfus Foundation and the National Science Foundation (Grant USE- 9150484) for financial support.
the pores are extremely small and evenly spread. The indi- vidual silica particles cannot be resolved. Hence, light inci- ~i~~~~~~~~ cited dent on these gels is mostly transmitted through the solid, and the gels are observed to be transparent. 1. Brinker, C. J.; Seherer, G. W. S o l 4 1 Scm-;Academic, 1990.
2. Klein, L. C. "Sol4el R o w i n g of SSlieates":Ann. RPu. Mabr Sci. 1985,15, 227. The xerogels are and the in- % Hmch, L L; West, J. K T h e S014dPrmed: Chem. Rev. ISM, 9O,8%72.
dividual silica particles may be resolved (-10 nm). They , ,eSR,, ,c hem,qoJ Silim;Wfiey:New 1979 are less packed than in the acid-eatal~zed ex- 5. Teichner. S. J.: Nieohn, G. A,; Rcsrini, M. A ; Gsrdes, G. E. E. Ad". Coll. ht Sci. amwle. Hence. lieht incident on the eels is reflected from 1 ~ 6 . 5 . 2 4 5 . . . the'solid, and the gels appear more oiaqne. 6. T~w&, P H . ; H w ~ , A . J.: ~ s . K . D . I ~ P , X . lst ht SW, ~ ~ ~ ~ a g o l ~ ; ~ r i ~ k ~
J., Ed.;Springw Pne. Phw.; Springer: Heidelberg, 1986; VoL 6, p 31.
Size and Complexity ofPolymers 7. P O ~ ~ ~ ~ L B . ; lbiehner, S. J. PW. tnt. congr. on cotalpis l m , z , 6 1 0 .
8. Klein, L. C. SalidSloBIonies 1989,32133, 639. Base catalysis favon rapid hydmlysis of silimn alkox-
,, h,,,R.w,d l,n~ip~sofSd4i~hnoio8y~hstihlteofMefakLon. ides compared to condensation. These conditions favor the don, 1989.
602 Journal of Chemical Education